General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.9 g/cm³ Show Material materials with Density of 8.9 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 205 GPa Show Material materials with Elastic modulus of 205 GPa |

100.0 °C | 200 GPa Show Material materials with Elastic modulus of 200 GPa | |

200.0 °C | 196 GPa Show Material materials with Elastic modulus of 196 GPa | |

300.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | |

400.0 °C | 182 GPa Show Material materials with Elastic modulus of 182 GPa | |

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | |

600.0 °C | 165 GPa Show Material materials with Elastic modulus of 165 GPa | |

700.0 °C | 153 GPa Show Material materials with Elastic modulus of 153 GPa | |

800.0 °C | 140 GPa Show Material materials with Elastic modulus of 140 GPa | |

900.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

Elongation | 20.0 °C | 35 - 40 % Show Material materials with Elongation of 35 - 40 % |

100.0 °C | 40 % Show Material materials with Elongation of 40 % | |

200.0 °C | 40 % Show Material materials with Elongation of 40 % | |

300.0 °C | 45 % Show Material materials with Elongation of 45 % | |

400.0 °C | 40 % Show Material materials with Elongation of 40 % | |

500.0 °C | 35 % Show Material materials with Elongation of 35 % | |

600.0 °C | 30 % Show Material materials with Elongation of 30 % | |

Unlock all property charts | ||

Elongation A100 | 20.0 °C | 20 - 30 % Show Material materials with Elongation A100 of 20 - 30 % |

Hardness, Brinell | 20.0 °C | 130 [-] Show Material materials with Hardness, Brinell of 130 [-] |

Tensile strength | 20.0 °C | 370 - 400 MPa Show Material materials with Tensile strength of 370 - 400 MPa |

100.0 °C | 390 MPa Show Material materials with Tensile strength of 390 MPa | |

200.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | |

300.0 °C | 370 MPa Show Material materials with Tensile strength of 370 MPa | |

400.0 °C | 330 MPa Show Material materials with Tensile strength of 330 MPa | |

500.0 °C | 255 MPa Show Material materials with Tensile strength of 255 MPa | |

600.0 °C | 200 MPa Show Material materials with Tensile strength of 200 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2 | 20.0 °C | 100 MPa Show Material materials with Yield strength Rp0.2 of 100 MPa |

100.0 °C | 150 MPa Show Material materials with Yield strength Rp0.2 of 150 MPa | |

200.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

300.0 °C | 140 MPa Show Material materials with Yield strength Rp0.2 of 140 MPa | |

400.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

500.0 °C | 100 MPa Show Material materials with Yield strength Rp0.2 of 100 MPa | |

600.0 °C | 80 MPa Show Material materials with Yield strength Rp0.2 of 80 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0 | 20.0 °C | 125 MPa Show Material materials with Yield strength Rp1.0 of 125 MPa |

100.0 °C | 180 MPa Show Material materials with Yield strength Rp1.0 of 180 MPa | |

200.0 °C | 160 MPa Show Material materials with Yield strength Rp1.0 of 160 MPa | |

300.0 °C | 170 MPa Show Material materials with Yield strength Rp1.0 of 170 MPa | |

400.0 °C | 160 MPa Show Material materials with Yield strength Rp1.0 of 160 MPa | |

500.0 °C | 130 MPa Show Material materials with Yield strength Rp1.0 of 130 MPa | |

600.0 °C | 105 MPa Show Material materials with Yield strength Rp1.0 of 105 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 100.0 °C | 1.33E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.33E-5 1/K | |

200.0 °C | 1.39E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.39E-5 1/K | ||

300.0 °C | 1.43E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.43E-5 1/K | ||

400.0 °C | 1.48E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.48E-5 1/K | ||

500.0 °C | 1.52E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.52E-5 1/K | ||

600.0 °C | 1.56E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.56E-5 1/K | ||

700.0 °C | 1.58E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.58E-5 1/K | ||

800.0 °C | 1.62E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.62E-5 1/K | ||

900.0 °C | 1.65E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 1/K | ||

1000.0 °C | 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.67E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1400 - 1500 °C Show Material materials with Melting point of 1400 - 1500 °C | Typical for Pure/Low Nickel Alloy | |

Specific heat capacity | 20.0 °C | 456 J/(kg·K) Show Material materials with Specific heat capacity of 456 J/(kg·K) | |

100.0 °C | 475 J/(kg·K) Show Material materials with Specific heat capacity of 475 J/(kg·K) | ||

200.0 °C | 500 J/(kg·K) Show Material materials with Specific heat capacity of 500 J/(kg·K) | ||

300.0 °C | 570 J/(kg·K) Show Material materials with Specific heat capacity of 570 J/(kg·K) | ||

400.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

500.0 °C | 525 J/(kg·K) Show Material materials with Specific heat capacity of 525 J/(kg·K) | ||

600.0 °C | 535 J/(kg·K) Show Material materials with Specific heat capacity of 535 J/(kg·K) | ||

700.0 °C | 550 J/(kg·K) Show Material materials with Specific heat capacity of 550 J/(kg·K) | ||

800.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

900.0 °C | 580 J/(kg·K) Show Material materials with Specific heat capacity of 580 J/(kg·K) | ||

1000.0 °C | 590 J/(kg·K) Show Material materials with Specific heat capacity of 590 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 70.5 W/(m·K) Show Material materials with Thermal conductivity of 70.5 W/(m·K) | |

100.0 °C | 66.5 W/(m·K) Show Material materials with Thermal conductivity of 66.5 W/(m·K) | ||

200.0 °C | 61.5 W/(m·K) Show Material materials with Thermal conductivity of 61.5 W/(m·K) | ||

300.0 °C | 57 W/(m·K) Show Material materials with Thermal conductivity of 57 W/(m·K) | ||

400.0 °C | 56 W/(m·K) Show Material materials with Thermal conductivity of 56 W/(m·K) | ||

500.0 °C | 57.5 W/(m·K) Show Material materials with Thermal conductivity of 57.5 W/(m·K) | ||

600.0 °C | 60 W/(m·K) Show Material materials with Thermal conductivity of 60 W/(m·K) | ||

700.0 °C | 62 W/(m·K) Show Material materials with Thermal conductivity of 62 W/(m·K) | ||

800.0 °C | 64 W/(m·K) Show Material materials with Thermal conductivity of 64 W/(m·K) | ||

900.0 °C | 66.5 W/(m·K) Show Material materials with Thermal conductivity of 66.5 W/(m·K) | ||

1000.0 °C | 69 W/(m·K) Show Material materials with Thermal conductivity of 69 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 9E-8 Ω·m Show Material materials with Electrical resistivity of 9E-8 Ω·m |

100.0 °C | 1.3E-7 Ω·m Show Material materials with Electrical resistivity of 1.3E-7 Ω·m | |

200.0 °C | 1.9E-7 Ω·m Show Material materials with Electrical resistivity of 1.9E-7 Ω·m | |

300.0 °C | 2.6E-7 Ω·m Show Material materials with Electrical resistivity of 2.6E-7 Ω·m | |

400.0 °C | 3.3E-7 Ω·m Show Material materials with Electrical resistivity of 3.3E-7 Ω·m | |

500.0 °C | 3.7E-7 Ω·m Show Material materials with Electrical resistivity of 3.7E-7 Ω·m | |

600.0 °C | 4E-7 Ω·m Show Material materials with Electrical resistivity of 4E-7 Ω·m | |

700.0 °C | 4.3E-7 Ω·m Show Material materials with Electrical resistivity of 4.3E-7 Ω·m | |

800.0 °C | 4.5E-7 Ω·m Show Material materials with Electrical resistivity of 4.5E-7 Ω·m | |

900.0 °C | 4.8E-7 Ω·m Show Material materials with Electrical resistivity of 4.8E-7 Ω·m | |

1000.0 °C | 5.1E-7 Ω·m Show Material materials with Electrical resistivity of 5.1E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.1 % Show Material materials with Carbon of 0.1 % |

Cobalt | 1 % Show Material materials with Cobalt of 1 % |

Copper | 0.25 % Show Material materials with Copper of 0.25 % |

Iron | 0.4 % Show Material materials with Iron of 0.4 % |

Magnesium | 0.15 % Show Material materials with Magnesium of 0.15 % |

Manganese | 0.35 % Show Material materials with Manganese of 0.35 % |

Nickel | 98.2 % Show Material materials with Nickel of 98.2 % |

Silicon | 0.25 % Show Material materials with Silicon of 0.25 % |

Sulfur | 5E-3 % Show Material materials with Sulfur of 5E-3 % |

Titanium | 0.1 % Show Material materials with Titanium of 0.1 % |